Designation: D1816 − 12
Standard Test Method for
Dielectric Breakdown Voltage of Insulating Liquids Using VDE Electrodes 1 This standard is issued under the ﬁxed designation D1816; the number immediately following the designation indicates the year of original origin al adoption or, in the case of revis revision, ion, the year of last revision. revision. A number in paren parenthese thesess indicates the year of last reappr reapproval. oval. A superscript epsilon (´) indicates an editorial change since the last revision or reapproval.
1. Sco Scope* pe*
2. Referenc Referenced ed Documents 2.1 ASTM Standards: 3 D235 Speciﬁ Speciﬁcation cation for Miner Mineral al Spirits (Petroleum Spirit Spirits) s) (Hydrocarbon Dry Cleaning Solvent) D923 Practices D923 Practices for Sampling Electrical Insulating Liquids D2225 Test D2225 Test Methods for Silicone Fluids Used for Electrical Insulation D2864 Termino erminology logy Relatin Relating g to Electric Electrical al Insu Insulating lating Liquids and Gases D3487 Spe Speciﬁ ciﬁcati cation on for Min Minera erall Ins Insulat ulating ing Oil Use Used d in Electrical Apparatus D4652 Speciﬁcation for Silicone Fluid Used for Electrical D4652 Insulation D6871 Speciﬁcation D6871 Speciﬁcation for Natural (Vegetable Oil) Ester Fluids Used in Electrical Apparatus 2.2 IEEE Standard: Standar Stan dard d 4 IEE IEEE E Stan Standar dard d Tech echniq niques ues for Hig High h Volta oltage ge 4 Testing C57.106 Guide C57.106 Guide for Acceptance and Maintenance of Insulating Oil in Equipment4
1.1 This test method covers covers the determination determination of the dielectric breakdown breakdown voltag voltagee of insulating liquids (oils of petro petroleum leum origin, silicone ﬂuids, high ﬁre-point mineral electrical insulating oils, synthetic ester ﬂuids and natural ester ﬂuids). This test method is applicable to insulating liquids commonly used in cables, transformers, oil circuit breakers, and similar apparatus as an insulating and coolin cooling g mediu medium. m. Refer to Termino erminollogy D2864 ogy D2864 for for deﬁnitions used in this test method. 1.2 This test method is sensitive sensitive to the deleter deleterious ious effects effects of moistu moi sture re in sol soluti ution on esp especia ecially lly whe when n cell cellulo ulosic sic ﬁbe ﬁbers rs are present in the liquid. It has been found to be especially useful in dia diagno gnostic stic and lab labora orator tory y inv investi estigat gation ionss of the die dielect lectric ric breakdown strength of insulating liquid in insulating systems. 2 1.3 This test method method is used to judge if the VDE electrode breakdown voltage requirements are met for insulating liquids. This test method should be used as recommended by professional organization standards such as IEEE C57.106. 1.4 Thi Thiss tes testt met method hod may be use used d to obtain the dielectri dielectricc breakdown of silicone ﬂuid as speciﬁed in Test Method D2225 Method D2225 and Speciﬁcation D4652 D4652,, provided that the discharge energy into the sample is less than 20 mJ (milli joule) per breakdown for ﬁve consecutive breakdowns. 1.5 Both the metric and the alternative alternative inch-pound inch-pound units units are acceptable. standard d doe doess not purport purport to add addre ress ss all of the 1.6 This standar safet sa fetyy co conc ncer erns ns,, if an anyy, as asso socia ciate ted d wit with h its us use. e. It is th thee responsibility of the user of this standard to establish appro priate safety and health practices and determine the applicability of regulatory limitations prior to use.
3. Signi Signiﬁcanc ﬁcancee and Use 3.1 The dielectric dielectric breakdown breakdown voltage of an insulating liquid is of im impo port rtan ance ce as a me meas asur uree of th thee li liqu quid id’s ’s ab abil ilit ity y to withstand electric stress without failure. The dielectric breakdown voltage serves to indicat indicatee the presence of contam contaminatin inating g agents age nts suc such h as wat water er,, dir dirt, t, cell cellulo ulosic sic ﬁbe ﬁbers, rs, or con conduc ductin ting g particles in the liquid, one or more of which may be present in signiﬁcant signiﬁ cant concen concentration trationss when low break breakdown down voltages are obtained. However, a high dielectric breakdown voltage does not necessarily indicate the absence of all contaminants; it may merely indicate that the concentrations of contaminants that are pres pr esen entt in th thee liq liqui uid d be betw tween een th thee ele electr ctrod odes es ar aree no nott lar large ge enough to deleteriously affect the average breakdown voltage of the liquid when tested by this test method (see Appendix X1..) X1
Thiss tes Thi testt met method hod is und under er the jur jurisd isdict iction ion of AST ASTM M Com Commit mittee tee D27 on Electrical Insulating Liquids and Gasesand is the direct responsibility of Subcommittee D27.05 mittee D27.05 on on Electrical Test. Curren Cur rentt edi editio tion n app approv roved ed Jun Junee 15, 201 2012. 2. Pub Publis lished hed Jul July y 201 2012. 2. Ori Origin ginall ally y approved approv ed in 1960 as D1816 – 60 60 T. Last previous edition approved in 2004 as D1816 – 04. DOI: 10.1520/D1816-12. 2 Supporting data is available from ASTM Headquarters. Request Request RR:D27-1006.
For referenced ASTM standards, visit the ASTM website, www.astm.org, or contact ASTM Customer Service at [email protected]
For Annual Book of ASTM Standards volume information, refer to the standard’s Document Summary page on the ASTM website. 4 Available from the Institute of Electrical and Electronic Engineers, Inc., PO Box 1331, Piscataway, NJ 08855.
INTERNO Y EXCLUSIVO INEN *A Summary USO of Changes section appears at the end of this standard USUARIO: ING. RONALD CHICAIZA
Copyright © ASTM International, 100 AUTORIZACI Barr Harbor Drive,ÓN PO Box C700, West Conshohocken, PA 19428-2959. States AUTORIZACIÓN A USUARIO ÚNICO, PROHIBIDA SUUnited REPRODUCCIÓN, REPRODUCCI ÓN,
Copyright by ASTM Int'l (all rights reserved); Tue Oct 22 16:50:07 EDT 2013 1 Downloaded/printed by (Ecuador MOU) pursuant to License Agreement. No further reproductions authorized.
D1816 − 12 3.2 This test method is used in laboratory or ﬁeld tests. For ﬁeld breakdown results to be comparable to laboratory results, all criteria including room temperature (20 to 30°C) must be met. 4. Electrical Apparatus 4.1 In addition to this section, use IEEE Standard 4 to determine other requirements necesary for conducting test measurements, and maintaining error limits using alternating voltages. Procedures to ensure accuracy should follow the requirements of IEEE Standard 4. Calibration(s) shall be traceable to national standards and calibration should be veriﬁed annually or more often to ensure accuracy requirements. IEEE Standard 4 is required during the manufacturing of the test apparatus and utilized during calibration of the equipment. 4.1.1 Test Voltage— The test voltage shall be an alternating voltage having a frequency in the range from 45 to 65 Hz, normally referred to as power-frequency voltage. The voltage wave shape should approximate a sinusoid with both half cycles closely alike, and it should have a ratio of peak-to-rms values equal to the square root of 2 within 65 %. 4.1.2 Generation of the Test Voltage— The test voltage is generally supplied by a transformer or resonant circuit. The voltage in the test circuit should be stable enough to be unaffected by varying current ﬂowing in the capacitive and resistive paths of the test circuit. Non-disruptive discharges in the test circuit should not reduce the test voltage to such an extent, and for such a time, that the disruptive discharge (breakdown) voltage of the test specimen is signiﬁcantly affected. In the case of a transformer, the short-circuit current delivered by the transformer should be sufficient to maintain the test voltage within 3 % during transient current pulses or discharges, and a short circuit current of 0.1 A may suffice. 4.1.3 Disruptive Voltage Measurement— Design the measurement circuit so the voltage recorded at the breakdown is the maximum voltage across the test specimen immediately prior to the disruptive breakdown, with an error no greater than 3 %.
4.4 Measuring Systems— The voltage shall be measured by a method that fuﬁlls the requirements of IEEE Standard No. 4, giving rms values. 4.5 Connect the electrode such that the voltage measured from each electrode with respect to ground during the test is equal within 5 %. 4.6 Accuracy— The combined accuracy of the voltmeter and voltage divider circuit shall be such that measurement error does not exceed 3 % at the rate-of-voltage rise speciﬁed in 4.3. For equipment manufactured prior to 1995 the maximum allowable error is 5 %. 5. Electrodes 5.1 The electrodes shall be polished brass sphericallycapped electrodes of the VDE (Verband Deutscher Elektrotechniker, Speciﬁcation 0370) type having the dimensions shown in Fig. 1 61 %, mounted with axes horizontal and coincident within 61 mm. 6. Test Cell 6.1 The test cell shall be designed to permit easy removal of the electrodes for cleaning and polishing, veriﬁcation that the shape is within the speciﬁed tolerance, and to permit easy adjustment of the gap spacing. The vector sum of the resistive and capacitive current of the cup, when ﬁlled with oil meeting the requirements of Speciﬁcation D3487, shall be less than 200 µA at 20 kV, at power frequency. Mount the electrodes rigidly from opposite sides with the spacing axially centered within 61 mm. Clearance from the electrodes to all sides, bottom, cover or baffle, and any part of the stirring device is at least 12.7 mm ( 1 ⁄ 2 in.). Provide the test cell with a motor-driven two-bladed impeller and drive shaft, constructed of a material having high dielectric strength. The two-bladed impeller is 35 mm (13 ⁄ 8 in.) 65 % between the blade extremities, having a pitch of 40 mm (1.57 in.) 65 % (blade angle of twenty degrees
4.2 Circuit-Interrupting Equipment— Design the circuit used to interrupt the disruptive discharge through the specimen to operate when the voltage across the specimen has collapsed to less than 100 V. It is recommended that the circuit design limit the disruptive current duration and magnitude to low values that will minimize damage to the electrodes and limit formation of non-soluble materials resulting from the breakdown, but consistent with the requirements of 4.1.2, but in no case should the short-circuit current exceed 1 mA/kV of applied voltage. 4.3 Voltage Control Equipment— Use a rate of voltage rise of 0.5 kV/s. The tolerance of the rate of rise should be 5 % for any new equipment manufactured after the year 2000. Automatic equipment should be used to control the voltage rate of rise because of the difficulty of maintaining a uniform voltage rise manually. The equipment should produce a straight-line voltage-time curve over the operating range of the equipment. INTERNO Y EXCLUSIVO INEN Calibrate and label automatic controls in termsUSO of rate-of-rise.
FIG. 1 VDE Electrode
USUARIO: ING. RONALD CHICAIZA AUTORIZACIÓN A USUARIO ÚNICO, PROHIBIDA SU REPRODUCCIÓN, 2017-02-08
Copyright by ASTM Int'l (all rights reserved); Tue Oct 22 16:50:07 EDT 2013 2 Downloaded/printed by (Ecuador MOU) pursuant to License Agreement. No further reproductions authorized.
D1816 − 12 (20°) 6 5 %), operating at a speed between 200 and 300 rpm. The impeller, located below the lower edge of the electrodes, rotates in such a direction that the resulting liquid ﬂow is directed downward against the bottom of the test cell. Construct the test cell of a material of high dielectric strength, that is not soluble in or attacked by any of the cleaning or test liquids used, and is nonabsorbent to moisture and the cleaning and test liquids. So that the breakdown may be observed, transparent materials are desirable, but not essential. In order to preclude stirring air with the sample, provide the cell with a cover or baffle that will effectively prevent air from contacting the circulating liquid. 7. Adjustment and Care of Electrodes and Test Cell 7.1 Electrode Spacing— With the electrodes held ﬁrmly in place, check the electrodes with a standard round gage for 2 6 0.03-mm (0.079-in.) spacing. If a dielectric breakdown does not occur during any of the consecutive breakdown tests using the 2 mm spacing or the sample is not adequate for the 2 mm spacing test cell a 1 6 0.03-mm (0.039-in.) spacing should be used to determine the breakdown voltage and the spacing reported. Flat “go” and “no-go” gages may be substituted having thicknesses of the speciﬁed value 60.03 mm for electrode spacing of 1 or 2 mm. If it is necessary to readjust the electrodes, set the electrodes ﬁrmly in place and check the spacing. For referee tests or tests that will be used for close comparisons, the laboratories shall agree in advance on the spacing for the tests and ensure that all other requirements of this test method are met. The spacing agreed upon shall be measured with the gage that corresponds exactly to the selected spacing within tolerance stated above for the gage. 7.2 Cleaning— Wipe the electrodes and cell clean with dry, lint-free tissue paper, or a clean dry chamois. It is important to avoid touching the electrodes or the cleaned gage with the ﬁngers or with portions of the tissue paper or chamois that have been in contact with the hands. After adjustment of the spacing, rinse the cell with a dry hydrocarbon solvent, such as kerosine or solvents of Speciﬁcation D235. Do not use a low boiling point solvent, as its rapid evaporation may cool the cell, causing moisture condensation. If this occurs, before using, warm the cell to evaporate the moisture. Avoid touching the electrodes or the inside of the cell after cleaning. After thorough cleaning, ﬂush the cell with new insulating liquid of the type to be tested that is ﬁltered through a 5-micron ﬁlter or smaller and containing less than 25 ppm moisture. Conduct a voltage breakdown test on a specimen of this insulating liquid in the manner speciﬁed in this test method. If the breakdown voltage is in the expected range for this conditioned insulating liquid, the cell is considered properly prepared for testing other samples. A lower than anticipated value is considered as evidence of cell contamination; then repeat the cleaning and the breakdown test with clean dry insulating liquid.
a 5-micron ﬁlter and containing less than 25 ppm moisture before testing the next specimen. When not in use, keep the cell ﬁlled with oil that meets the requirements of Speciﬁcation D3487 of the type normally tested. Alternatively, the cell may be stored empty in a dust-free cabinet. At the beginning of each days testing, clean according to 7.2. 7.4 Polishing of Electrodes— When electrodes show slight etching, scratching, pitting, or carbon accumulation, they should be removed from the test cup and polished by buffing with jeweler’s rouge using a soft cloth or soft buffing wheel. The residue from the buffing should be removed by repeated wiping with lint-free tissue paper saturated with a suitable solvent, followed by solvent rinsing or ultrasonic cleaning. After careful inspection, any electrodes from which pitting cannot be removed by light buffing should be discarded, as more reﬁnishing would destroy the electrode contour and dimensions shown in Fig. 1. Reinstall the electrodes in the test cup and adjust spacing and clean in accordance with 7.1 and 7.2. 8. Sampling 8.1 Obtain a sample of the insulating liquid to be tested using appropriate ASTM sampling apparatus. Insulating liquid sampling procedures are detailed in Practice D923. Particular reference should be made to the general precaution statement of this test method. The sample shall be taken in a dry, clean, non-permeable bottle. Tightly seal and shield from light until ready to be tested. Plastic bottles are permeable and moisture content of the sample may change resulting in a measurable difference when compared to samples collected in nonpermeable containers. Prior to starting the test, the sample shall be inspected for the presence of moisture, sludge, metallic particles, or other foreign matter. If the sample shows evidence of free water, the dielectric breakdown test should be waived, and the sample reported as unsatisfactory. 9. Test Procedure 9.1 Allow the sample and the test cup to equilibrate to ambient temperature. Laboratory and referee tests shall be conducted at room temperature (20 to 30°C). 9.2 To ensure a homogenous sample, gently invert and swirl the sample container several times. Rapid agitation is undesirable, since an excessive amount of air may be introduced into the liquid. Within 1 min after agitation, use a small portion of the sample to rinse the test cell. Drain the rinse. Within 30 s of the rinse, ﬁll the cell slowly with the remaining portion of the sample. The cell is full when closing the cover or baffle allows no air to be in contact with the insulating liquid.
9.3 Wait at least 3 min but no more than 5 min between ﬁlling the cup and application of voltage for the ﬁrst breakdown. For high ﬁre-point electrical insulating oils, natural esters and synthetic esters, the hold time before the initial 7.3 Daily Use— At the beginning of each day’s testing, the application of voltage shall be at least 30 min. Apply the electrodes shall be examined for pitting and carbon accumulavoltage increasing from zero at the rate of 0.5 kV/s 6 5 % until tion, and the spacing checked. If the test of any sample is below breakdown occurs as indicated by operation of the circuitthe breakdown value being used by the operator as a minimum interrupting equipment; record the highest rms voltage value satisfactory value, drain the cell and ﬂush the cell with new that occurred immediately prior to each breakdown. OccaUSO INTERNO Y EXCLUSIVO INEN insulating liquid of the type to be tested that is ﬁltered through sional momentary discharges may occur which do not result in USUARIO: ING. RONALD CHICAIZA AUTORIZACIÓN A USUARIO ÚNICO, PROHIBIDA SU REPRODUCCIÓN, 2017-02-08
Copyright by ASTM Int'l (all rights reserved); Tue Oct 22 16:50:07 EDT 2013 3 Downloaded/printed by (Ecuador MOU) pursuant to License Agreement. No further reproductions authorized.
D1816 − 12 operation of the interrupting equipment; these shall be disregarded until the voltage across the specimen collapses to less than 100 V. Conduct four additional breakdowns waiting at least 60 s but no more than 90 s before applications of voltage for successive breakdowns. (During the intervals before voltage application, between breakdowns, and at the time voltage is being applied, the propeller shall be circulating the insulating liquid.)
10.1.2 The volts (rms value) at each breakdown, and the mean of all breakdowns reported to two signiﬁcant digits,
9.4 Calculate the mean of the ﬁve breakdowns as follows:
11.1 Single-Operator Precision— The single operator percent coefficient of variance of a single test result comprised of 5 breakdowns has been found for the 1 mm gap to be 14 % and for the 2 mm gap 11 %. Therefore, results of two properly conducted tests by the same operator on the same sample should not differ by more than 40 % and 30 % respectively. The maximum allowable range for the series of 5 breakdowns should not exceed 120 % for the 1 mm gap and 92 % for the 2 mm gap.
¯ 5 X
( X i
where: ¯ X = mean of the ﬁve individual values, X i = ith breakdown voltage. 9.5 Using the breakdown voltage values determined in 9.3, determine that the range of the ﬁve (5) breakdown voltages does not exceed the values indicated as follows: Range
X Hi gh es t
X Lo we st
where: X Highest = the highest breakdown voltage of the ﬁve readings, and X Lowest = the lowest breakdown of the ﬁve readings. 1 mm gap setting 2 mm gap setting
Range must be less than 120 % of the mean of the ﬁve (5) breakdown voltages Range must be less than 92 % of the mean of the ﬁve (5) breakdown voltages
If this range is exceeded and there is sufficient volume of test specimen, repeat the analysis on a new cup ﬁlling. If an insufficient volume of test specimen is available, the test result can be reported with an additional comment that the range of the breakdowns exceeds the allowable range. 9.6 When it is desired merely to determine if the dielectric strength is above or below a speciﬁed level, ﬁve breakdowns are required, provided the ﬁve values are all above or all below this level. Otherwise, follow the procedure described in 9.3-9.5
10.1.3 The approximate temperature of the insulating liquid at the time of the test, and 10.1.4 The electrode spacing. 11. Precision and Bias5
11.2 Multilaboratory Precision— The multilaboratory percent coefficient of variance has been found for the 1 mm gap to be 17 % and for the 2 mm gap 14 %. Therefore, two separate test results conducted by separate laboratories on the same sample of insulating liquid should not differ by more than 47 % of the mean of the two tests if the 1 mm gap was used or differs by more than 40 % of the mean of the two tests if the 2 mm gap was used. The precision statement for the 1 mm gap is temporary, because sufficient laboratories were not available and testing is planned to replace the precision statement before 2009. 11.3 Bias— No statement can be made about the bias of this test method because a standard reference material is not available. 12. Keywords 12.1 breakdown voltage; dielectric strength; insulating liquids; insulating oils; test cell; VDE electrodes
10. Report 10.1 Include in the report the following: 10.1.1 The test method used,
Supporting data is available from ASTM International Headquarters. Request RR:D27-1014.
APPENDIX (Nonmandatory Information) X1. FACTORS THAT AFFECT THE DIELECTRIC BREAKDOWN VOLTAGE OF INSULATING LIQUIDS AT COMMERCIAL POWER FREQUENCIES
X1.1 The dielectric breakdown voltage of an insulating liquid at commercial power frequencies is also affected by:
X1.1.5 Water content of the insulating liquid, X1.1.6 Size and number of particles in the insulating liquid,
X1.1.1 The degree of uniformity of the electric ﬁeld, X1.1.2 The area of the electrodes, X1.1.3 Volume of the insulating liquid under maximum stress, X1.1.4 Insulation on the electrodes,
X1.1.7 Length of time for which the insulating liquid is under stress,
X1.1.8 The temperature of the insulating liquid as it affects the relative USO INTERNO Y EXCLUSIVO INENsaturation level of moisture in solution,
USUARIO: ING. RONALD CHICAIZA AUTORIZACIÓN A USUARIO ÚNICO, PROHIBIDA SU REPRODUCCIÓN, 2017-02-08
Copyright by ASTM Int'l (all rights reserved); Tue Oct 22 16:50:07 EDT 2013 4 Downloaded/printed by (Ecuador MOU) pursuant to License Agreement. No further reproductions authorized.
D1816 − 12 X1.1.9 Gassing tendencies of the insulating liquid under the inﬂuence of electric stress, X1.1.10 Concentration of dissolved gases if saturation levels are exceeded as a result of a sudden cooling or decrease in pressure, which may cause the formation of gas bubbles, X1.1.11 Incompatibility with materials of construction, and X1.1.12 Velocity of ﬂow. X1.1.13 A decrease in dielectric strength of the insulating liquid can have an accentuated effect on the electric creepage strength of the solid insulating materials immersed in the insulating liquid.
X1.2 Because of the separate, cumulative, and in some cases, interacting effects of the inﬂuences listed above, the average breakdown voltage of a liquid as determined by this test method cannot be used directly for design purposes. Procedures utilizing electrode shapes and conﬁgurations similar to those used in insulating liquid ﬁlled apparatus are used to determine design data and to study the inﬂuence of the variables. However, test results utilizing the rounded electrodes in this test method do give an indication of the relative dielectric strength of the insulating liquid in the insulation system.
SUMMARY OF CHANGES Committee D27 has identiﬁed the location of selected changes to this standard since the last issue (D1816-04) that may impact the use of this standard. (1) Revised title to include other insulating liquids (silicone ﬂuids, natural and synthetic esters). (2) Changed the volume requirement for the test cell in 6.1. (3) Added Requirements for handling samples containing free water in 8.1. (4) Added hold time for testing natural and synthetic esters and high ﬁre point ﬂuids in 9.3.
(5) Removed the standard deviation calculation and added Range calculation in 9.4 and 9.5. (6) Added Instructions for handling test results when they exceed the allowable range and there is insufficient sample to retest.
ASTM International takes no position respecting the validity of any patent rights asserted in connection with any item mentioned in this standard. Users of this standard are expressly advised that determination of the validity of any such patent rights, and the risk of infringement of such rights, are entirely their own responsibility. This standard is subject to revision at any time by the responsible technical committee and must be reviewed every ﬁve years and if not revised, either reapproved or withdrawn. Your comments are invited either for revision of this standard or for additional standards and should be addressed to ASTM International Headquarters. Your comments will receive careful consideration at a meeting of the responsible technical committee, which you may attend. If you feel that your comments have not received a fair hearing you should make your views known to the ASTM Committee on Standards, at the address shown below. This standard is copyrighted by ASTM International, 100 Barr Harbor Drive, PO Box C700, West Conshohocken, PA 19428-2959, United States. Individual reprints (single or multiple copies) of this standard may be obtained by contacting ASTM at the above address or at 610-832-9585 (phone), 610-832-9555 (fax), or [email protected]
(e-mail); or through the ASTM website (www.astm.org). Permission rights to photocopy the standard may also be secured from the ASTM website (www.astm.org/ COPYRIGHT/).
USO INTERNO Y EXCLUSIVO INEN USUARIO: ING. RONALD CHICAIZA AUTORIZACIÓN A USUARIO ÚNICO, PROHIBIDA SU REPRODUCCIÓN, 2017-02-08 Copyright by ASTM Int'l (all rights reserved); Tue Oct 22 16:50:07 EDT 2013 5 Downloaded/printed by (Ecuador MOU) pursuant to License Agreement. No further reproductions authorized.